24Some examples of composite materials: (a) plywood is a laminar composite of layers of wood veneer, (b) fiberglass is a fiber-reinforced composite containing stiff, strong glass fibers in a softer polymer matrix ( 175), and (c) concrete is a particulate composite containing coarse sand or gravel in a cement matrix (reduced 50%).
58Failure mechanismsFailure in fibers (ductile-matrix composites, e.g., polymer-matrix and metal-matrix composites), so a high interfacial strength is desired.Failure in matrix (brittle-matrix composites, e.g., ceramic-matrix and carbon-matrix composites), so a low interfacial strength is desired (to allow cracks to deflect along fiber-matrix interface, thereby allowing fibers to pull out for the purpose of increasing the toughness)
60Two failure modes in ceramic-ceramic composites: (a) Extensive pull-out of SiC fibers in a glass matrix provides good composite toughness (x20). (b) Bridging of some fibers across a crack enhances the toughness of a ceramic-matrix composite (unknown magnification).
63Reasons for fiber-matrix interface engineering To control fiber-matrix bond strength (shear bond strength)To improve wetting of matrix precursor on fiberTo improve fiber dispersion
64Methods for fiber-matrix interface engineering Fiber surface treatmentDispersant as an additive to the matrix
65Methods of fiber surface treatment Chemical treatment fiberCoating of fiber
66All liquid treatments at reflux temperature. Fiber properties Table 2.2 Effects of various surface treatments on properties of high-modulus carbon fibers and their epoxy-matrix composites.All liquid treatments at reflux temperature.Fiber propertiesComposite propertiesFiber treatmentWt. loss(%)Tensile strength loss (%)Flexural strength loss (%)ILSS gain (%)400ºC in air (30 min)18500ºC in air (30 min)0.461250600ºC in air (30 min)4.5Too weak to test-60% HNO3 (15 min)0.28115.25% NaOCl (30 min)1.553010-15% NaOCl (15 min)15% HClO4 (15 min)5% KMnO4/10% NaOH (15 min)15195% KMnO4/10% H2SO4 (15 min)6.0(+)17139510% H2O2/20% H2SO4 (15 min)0.11442% HNO3/30% H2SO4 (15 min)4(+)10% NaClO3/15% NaOH (15 min)10% NaClO3/25% H2SO4 (15 min)25(+)9115% NaClO3/40% H2SO4 (15 min)0.7410810% Na2Cr2O7/25% H2SO4 (15 min)0.315(+)15% Na2Cr2O7/40% H2SO4 (15 min)1.72731
67Types of polymer-matrix composites Thermoplastic-matrix compositesThermoset-matrix composites
68Lower manufacturing cost of thermoplastic-matrix composites no cureunlimited shelf-lifereprocessing possible (for repair and recycling)less health risks due to chemicals during processinglow moisture contentthermal shaping possibleweldability (fusion bonding possible)
69Better performance of thermoplastic-matrix composites high toughness (damage tolerance)good hot/wet propertieshigh environmental tolerance
70Disadvantages of thermoplastic-matrix composites limitations in processing methodshigh processing temperatureshigh viscositiesprepreg (collection of continuous fibers aligned to form a sheet which has been impregnated with the polymer or polymer precursor) being stiff and dry when solvent is not used (i.e., not drapeable or tacky)fiber surface treatments less developed
71Attractive properties of carbon fiber polymer-matrix composites low density (40% lower than aluminum)high strength (as strong as high-strength steels)high stiffness (stiffer than titanium, yet much lower in density)good fatigue resistance (a virtually unlimited life under fatigue loading)good creep resistance
72Attractive properties of carbon fiber polymer-matrix composites low friction coefficient and good wear resistance (a 40 wt.% short carbon fiber nylon-matrix composite has a friction coefficient nearly as low as Teflon and unlubricated wear properties approaching those of lubricated steel)toughness and damage tolerance (can be designed by using laminate orientation to be tougher and much more damage tolerant than metals)chemical resistance (chemical resistance controlled by the polymer matrix)corrosion resistance (impervious to corrosion)
73Attractive properties of carbon fiber polymer-matrix composites dimensional stability (can be designed for zero coefficient of thermal expansion)vibration damping ability (excellent structural damping when compared with metals)low electrical resistivityhigh electromagnetic interference (EMI) shielding effectivenesshigh thermal conductivity
74Limitation of polymer-matrix composites Inability to resist high temperatures
75Carbon-matrix composites Ability to resist high temperatures
76Carbon-carbon (C/C) composites Carbon fiberCarbon matrixCarbon matrix made from pitch or polymer
110Methods of making carbon-carbon composites Carbonization, followed by impregnation of pitch or resin, and repeating the carbonization-impregnation process again and again until sufficient density has been attained.Chemical vapor infiltration (CVI) using a carbonaceous gas, i.e., CVD under a temperature/pressure gradient so as to prevent crust formation, thereby allowing complete infiltration; CVI can be an extra step that follows carbonization-impregnation for the purpose of filling the pores.
112Grades of pitch Isotropic pitch Mesophase pitch (liquid crystal form called the mesophase)
113Main problem with carbon-carbon composites Oxidation at high temperatures in the presence of oxygen
114Methods for oxidation protection of carbon-carbon composites up to 1700C SiC conversion coatingOxidation inhibitorsGlassy sealantDense SiC or Si3N4 overlayer on glassy sealant or SiC conversion coating
115SiC conversion coating method SiC coating (known as SiC conversion coating, due to graded composition from pure SiC at the surface to pure carbon inside)
116Methods of applying SiC conversion coating - Pack cementation,- Reaction sintering,- Silicone resin impregnation/pyrolysis, or- Chemical vapor deposition (CVD) to the outer surface of the composite.
117Pack cementationPacking the composite in a mixture of SiC and Si powders and heat up to 1600°CChemical conversion of the outermost surfaceof the composite to SiCSiC coating thickness typically mm.
118Si(l) + C SiC Si(g) + C SiC SiO(g) + 2C SiC + CO(g) Pack cementationSi(l) + C SiCSi(g) + C SiCSiO(g) + 2C SiC + CO(g)Problem with entrapped silicon vaporising.
119Reaction sinteringDipping C/C composite into a suspension of Si powder (10 μm) in an alcohol solution and then sintering at 1600°C for 4 hours in argon.
120Silicone resin impregnation/pyrolysis Vacuum impregnation and cold isostatic pressing (30,000 psi or 200 MPa) a silicone resin into the matrix of a C/C composite and subsequent pyrolysis at 1600°C for 2 hours in argon.Note: Silicone is a polymer with silicon atoms as a part of the backbone.
121Prior deposition of carbon film (10 μm) by CVD Prior to pack cementation, reaction sintering or resin impregnationTo improve homogeneity of C/C surfaceTo ease the reaction with Si
122Dense SiC or Si3N4 overlayers SiC overlayer is more dense than the SiC conversion coating.As oxygen barrierTo control venting of reaction products to the outsideMade by chemical vapor deposition (CVD)
123CH3SiCl3(g) SiC + 3HCl(g) Chemical vapor deposition (CVD)by thermal decompositionof a volatile silicon compoundHeat/H2CH3SiCl3(g) SiC + 3HCl(g)Temperature: 1125°C
124SiSiC overlayerCVD overlayer contains a small percentage of unreacted silicon dispersed in the SiC,The excess Si upon oxidation becomes SiO2, which has a very low oxygen diffusion coefficient.
125Advantages of SiC or Si3N4 Thermal expansion compatibility with C/CLow oxidation rateThin amorphous SiO2 scale that grows has low oxygen diffusion coefficient.
126SiC or ineffective above 1800°C Reactions at the interface between SiO2 and SiC or Si3N4Reduction of SiO2 by carbon to form CO gas.
127Oxygen inhibitors Oxygen getters Glass formers To provide additional oxidation protection from within by migrating to the outer surface and sealing cracks and voids during oxidation.
128Examples of inhibitors Elemental Si, Ti and BSiC, Ti5Si3 and TiB2Alloys such as Si2TiB14Organoborosilazane polymer solutionOxidation of the elemental Si, Ti or B within the carbon matrix forms a viscous glass, which serves as a sealant that flows into the microcracks of the SiC coating.
129Boron as an oxidation inhibitor Boron is oxidized to form B2O3.B2O3 blocks active sites, such as the edge carbon atoms.B2O3 forms a mobile diffusion barrier for oxygen.
131Inhibition factorRatio of oxidation rate of untreated carbon to that of the treated carbon
132Incorporating particulate fillers in the resin or pitch Method of introducing oxidation inhibitors to the carbon matrixIncorporating particulate fillers in the resin or pitch(i) prior to prepregging. during lay-up and(ii) during densification cycles.
133Glassy sealantsGlazes comprising mainly silicates (SiOx) and borates (B2O3).Glaze can be filled with SiC particlesParticularly important if the SiC conversion coating is porousGlaze fills microcracks in the dense overlayer
134Application of a glassy sealant on top of the SiC conversion coating mainly by slurry brush-on, so that the sealants melt, fill voids and stop oxygen diffusion, and, in some cases, act as oxygen getters.
135Effectiveness of borate sealants Borates wet C and SiC quite wellBorates cannot be used above 1200°C due to volatilizationBorates have poor moisture resistance due to hydrolysis, which results in swelling and crumblingBorate has a tendency to galvanically corrode SiC coatings at high temperatures
136Modified borate sealants The problems of borate can be alleviated by using multicomponent systems such as 10TiO2.20SiO2.70B2O3 .TiO2 has a high solubility in B2O3 and is used to prevent the volatilization of B2O3 and increase the viscosity.SiO2 acts to increase the moisture resistance, reduce B2O3 volatility, increase viscosity and prevent corrosion of SiC by B2O3.
137Dense SiC or Si3N4 overlayer Applied by CVD.On top of glassy sealant or on top of SiC conversion coatingTo control and inhibit transfer of oxygen to the substrateTo control the venting of reaction products to the outside
138Method of oxidation protection of C/C above 1700°C Four-layer coating scheme:(1) Refractory oxide (e.g., ZrO2, HfO2, Y2O3, ThO2) as the outer layer for erosion protection.(2) SiO2 glass inner layer as and oxygen barrier and sealant.(3) Another refractory oxide layer for isolation of the SiO2 from the carbide layer underneath.(4) Refractory carbide layer (e.g., TaC, TiC, HfC, ZrC) to interface with the C/C substrate and to provide a carbon diffusion barrier
140Fundamental approaches for oxidation protection of carbons Prevention of catalysisRetardation of gas access to the carbonInhibition of carbon-gas reactionsImprovement in the carbon crystalline structure
141Carbon matrix precursors Pitch (preferred for oxidation protection)Chemical vapor infiltration (CVI) carbon (preferred for oxidation protection)Resins (not preferred for oxidation protection)
142Effects of carbon fiber on oxidation protection Alignment of the matrix molecules near the fibersMicrostructure of fiber affecting that of matrixMicrostructure of matrix affecting amount of accessible porosity in the matrix
143Disadvantage of coatings on C/C Degrade room temperature mechanical properties of C/C
144Metal-matrix composites Better temperature resistance than polymer-matrix compositesLower temperature resistance than ceramic-matrix compositesHigh fabrication cost compared to polymer-matrix compositesLow fabrication cost compared to ceramic-matrix composites
150Difficulty in liquid metal infiltation Liquid metal does not wet ceramic or carbon particles/fibers well.
151Reaction between metal and reinforcement Helps wettingDegrades reinforcementReaction product (e.g., a carbide) lining the metal-reinforcement interface may be brittle
152Methods of wetting enhancement Coat reinforcement with a metal (e.g., Ni, Cu, Ag) by platingCoat reinforcement with a ceramic (e.g., TiC, SiC, B4C, TiB2, TiN, K2ZrF6, ZrO2) by CVD, solution coating, etc.
153Coating of TiB2 on carbon fiber by CVD TiCl4 and BCl3 gases, which are reduced by zinc vaporCoating particularly good for liquid aluminum
154Solution coating method Dip in organometallic solution (e.g., alkoxides, which are M(OR)x, where M is the metal, and R is a hydrocarbon group, such as methyl, ethyl, etc.)Hydrolysis or pyrolysis to organometallic compounds